New fibrereinforced polymer box beam: investigation of static behaviour


 Angel West
 11 months ago
 Views:
Transcription
1 New fibrereinforced polymer box beam: investigation of static behaviour by Mario Springolo BE (Civil) (Hons I) A dissertation submitted for the award of DOCTOR OF PHILOSOPHY Faculty of Engineering and Surveying University of Southern Queensland M. Springolo Chapter 1 Page i
2 Abstract This thesis discusses the development of a new type of fibrereinforced polymer (FRP) beam for use in civil engineering systems. After a detailed evaluation of the advantages and disadvantages of current FRP beam technology, a different approach is proposed which combines traditional laminates with a novel casting technique. To predimension the beam, the classical beam theory is adapted to allow for FRP materials. The resulting formulae were used to determine critical parameters, such as laminate thickness and location in the crosssection, and core dimensions, and to identify failure modes. Based on the results of this analytical study, a detailed testing program was developed. In addition to classical tests, such as bending, shear, and lateral torsion, the performance of the beam was also examined under particular loading regimes specifically designed to induce local failure modes, such as buckling of the web and bearing failure of the section under concentrated loads. The experimental results revealed very good agreement with the analytical predictions. These results were corroborated by a detailed nonlinear finiteelement analysis, including core cracking and laminate damage. This analysis, in particular, highlighted the synergy between bending and shear behaviour of the beam. This study has revealed that this new type of FRP beam behaves in a predictable manner. Furthermore, the experimental results verified that the crosssection, which combines traditional laminates with cast polymer concrete, did not suffer from many of the disadvantages identified in current FRP beams. The cracking of the polymer concrete under shear, however, does cause the beam to fail prior to the laminates reaching their ultimate shear stress. M. Springolo Page ii
3 Certification of Dissertation I certify that the ideas, experimental work, results, analysis and conclusions reported in this dissertation are entirely my own effort, except where otherwise acknowledged. I also certify that the work is original and has not been previously submitted for any other award, except where otherwise acknowledged / / Signature of Candidate Date Endorsed: / / Signature of Supervisor Date M. Springolo Page iii
4 Acknowledgements Prof. Gerard Van Erp my supervisor, for recognising the potential within myself and encouraging me to do this work Dr. Amar Kehanne my cosupervisor, for the support, encouragement, and critical review of this thesis and, for spending hours at a time working through this thesis with me. USQ workshop and technical staff for providing practical help with experimental test jigs and running experiments. The Fibre composites design and development team (FCDD) for providing the space and tools to produce the test specimens Karen my wife, for her constant and unwavering support while having to put up with my late nights at the Uni and in the study. God Without whom, nothing is possible. M. Springolo Page iv
5 Contents Chapter 1 Introduction Introduction Background Application of FRP in civil engineering systems Objective of the study Aim Scope Layout of the Thesis... 6 References... 7 Chapter 2 Overview of fibrereinforced polymer materials and their manufacture Introduction Background Constituents of fibrereinforced polymers Matrix General Thermosetting Unsaturated polyesters Epoxydes Vinylester Other thermosetting resins Thermoplastics Fibres General Inorganic Organic Carbon Aramid Other fibres Fibre forms for use in FRP Chopped strand (CSM) and Continuous strand (CCSM) mats Unidirectional mat (UD) Woven roving mat (WR) Biaxial (BA) and Doublebias (DB) mats M. Springolo Page v
6 Sizing Yarn Sizes Roving Sizes Filler materials Laminated fibrereinforced polymers and their properties Considerations for Laminate Layup Laminate terminology Manufacturing techniques Pultrusion Filamentwinding Injection moulding Hand and machine laminating Consolidation techniques Vacuum bagging Autoclave consolidation Conclusion References Chapter 3 Existing FRP beams: advantages and limitations Introduction Description and behaviour of FRP beams developed for civil engineering applications Commercially Available beams Pultruded beams Delamination due to radial stresses and associated flange buckling Web buckling Connecting pultruded beams Limitations of the pultrusion process Recent improvement in pultruded section design Filamentwound beams Custom designed beams I beam with optimum fibre orientations Concept combining concrete and an FRP box beam Concretefilled tubes Concept combining a polymer core material and an FRP box beam Conclusion References M. Springolo Page vi
7 Chapter 4 State of the art in FRP beam analysis and design methodologies Introduction Analysis techniques for FRP beams From micro to macro mechanics Three dimensional analysis Twodimensional analysis Onedimensional analysis Flexure Stress versus strain Beam theory Determination of engineering constants Combination of material and section constants into one term Buckling Lateral torsional buckling Time effects Shortcomings of current methodologies used to determine FRP beam section size General Moment and shear Combined moment and shear Lateral torsional buckling Bearing capacity Creep and creep rupture Ductility Conclusion References Chapter 5 Conception of a new hybrid composite beam Introduction General Proposed solution to flange buckling and associated delamination at the webflange interface Control of web buckling Proposed solution to compressive failure under vertical loads Fibre orientation Description of the new beam Section Design M. Springolo Page vii
8 5.2.2 Determination of section size of test beams Span Selection of test beam depth Width Flange and web core dimensions Final beam dimensions Materials EGlass Laminate properties Core properties Production processes Material Use Production Summary References Chapter 6 Analytical modelling of the FRP beam behaviour Introduction Pure bending Moment curvature behaviour Uncracked beam behaviour Effects of cracking of the PFR material on the behaviour of the beam Effective stiffness of the beam Primary failure modes General Critical components Tensile failure of the bottom unidirectional laminate Compressive failure of the unidirectional laminate Predominant primary failure mode Secondary failure modes General Moment buckling of the webs Compression buckling of the top flange Web failures (a), (b) and (c) Compression buckling capacity of the webs (a) Crushing or tearing of the web (b) and (c) RHS laminate failure within the flanges (d) M. Springolo Page viii
9 Longitudinal cracking of the core in the flanges (e) and (f) Other failure modes Pure shear Sheardeformation behaviour Shear stress distribution Shearinduced failure modes Cracking of the core Shear failure of the webs Shear buckling of the webs Flange failure Momentshear interaction Deformation behaviour Shearmoment capacity General Principal stress determination (Mohr s circle) Empirical models Linear relationship (Eurocomp) Elliptical relationship (General) Comparison of models Lateral torsional resistance of the beam General Determination of the torsion constant Simplified analysis of lateral torsional buckling Analytical formulation of lateral torsional buckling behaviour Critical buckling moment formulae Generalised approach FRP beam Determination of the bearing stress distribution angle Key parameters Conclusions References Chapter 7 Experimental characterisation of the beam behaviour Introduction Strain distribution throughout the section Bending General M. Springolo Page ix
10 7.3.2 Beam tests Tensile failure of the unidirectional laminate Compressive failure of the unidirectional laminate Compression buckling of the top flange Longitudinal cracking of the core in the flanges Moment buckling of the webs Compression buckling of the webs Characterisation of the local bearing capacity Shear General Beam shear capacity Estimation of beam shear capacity by testing under combined moment and shear loading Determination of beam shear capacity by testing web specimens Comparison of results and the analytical solution for the pure shear capacity of the beam Shear buckling capacity of the webs Combined moment and shear Lateral torsional buckling Torsion constant Lateral torsional buckling behaviour Bearing stresses distribution angle Creep General Discussion Conclusions References Chapter 8 Nonlinear finite element modelling of the FRP beam behaviour Introduction Modelling the complex behaviour of the FRP beam Limitations of standard FE software Description of the FE models Modelling the FRP beam using Strand Modelling the FRP beam using ABAQUS Models under specific loading regimes General Moment buckling of the webs M. Springolo Page x
11 8.3.3 Compression buckling of webs Longitudinal cracking of the core in the flanges Shear Web shear strength Shear buckling of the webs Overall beam performance Combined moment and shear Lateral torsional buckling Torsion constant Lateral torsional buckling Conclusions References Chapter 9 Conclusions and recommendations Review of research Main findings Recommendations for further research Appendices Appendix A. Classical Laminate Theory References Appendix B. Production Process Preparation of unidirectional laminates Laying of the inner RHS laminates Provision of spacers Assembling the mould Pumping of PFR Laying the outer RHS laminates Curing the beams Appendix C. Theory C.1 Transformed section C.2 Poisson ratio of the FRP beam web C.3 Derivation of F w C.4 Flow chart of analytical program for pure bending C.5 Calculation of shear deformation C.6 Flow chart of analytical program for pure shear C.7 Flow chart of analytical program for combined shear and moment C.8 Analytical formulation of lateral torsional buckling behaviour M. Springolo Page xi
12 C.9 Flow chart of analytical program for torsion C.10 Flow chart of analytical program for lateral torsional buckling Appendix D. Experimentation D.1 Web buckling Appendix E. Results E.1 Beams in pure bending B4 (ms03b4) B5 (ms03b5) B6 (ms03b6) B7 (ms03b7) B8 (ms03b8) B9 (ms03b9) E.2 Web compression buckling E.3 Beam crushing E.4 Web shear capacity S1 (ms041) S2 (ms042) E.5 Beams under combined loading of moment and shear S1 (ms04b1) S2 (ms04b2) S3 (ms04b3) S4 (ms04b4) S5 (ms04b5) S6 (ms04b6) E.6 Beams under torsion loading Beams Tb1 and Tb E.7 Distribution angle E.8 Time effects: Shortterm failure load and deflection of the beams B1 (ms03b1) Appendix F. FEA F.1 Fortran program for damage analysis and material properties used by ABAQUS F.2 Damage and failure of a laminated composite plate References M. Springolo Page xii
13 Figures Figure 1.1 FRP pedestrian cable stay bridge across the River Tay in Aberfeldy, Scotland (Barbero 1998)... 3 Figure 1.2 Pedestrian bridge (Ashland Chemical Company 1997)... 4 Figure 1.3 Parson s Bridge, Ceredigion midwales (Strongwell Ltd. 2002)... 4 Figure 1.4 Vehicular bridge in the City of Hamilton, Butler County, Ohio (icivil)... 4 Figure 1.5 Ten metre vehicular bridge undergoing testing in Toowoomba, Queensland... 4 Figure 2.1 Reinforcement matrix interface Figure 2.2 Forms of reinforcement (not to scale) Figure 2.3 Unidirectional mat Figure 2.4 Woven roving mat Figure 2.5 Biaxial mat Figure 2.6 Doublebias mat Figure 2.7 Layers of plies that form a laminate Figure 2.8 Laminate designation [45/0/45/90/90/30] Figure 2.9 The pultrusion process (Fibreforce Composites Limited 2002) Figure 2.10 Filamentwinding technique (SaintGobain Vetrotex America International 2001) Figure 2.11 Injection moulding (Michigan State University 1999) Figure 2.12 Typical vacuum bagging Figure 3.1 Sea Life Park bridges, Hawaii (Strongwell Ltd. 2002) Figure 3.2 DURAGRID Phenolic Grating on an offshore platform (Strongwell Ltd. 2002) Figure 3.3 Delamination around curved regions Figure 3.4 Strongwell 36inch hybrid double web beam (Strongwell Ltd. 2002) Figure 3.5 Lee beam Figure 3.6 Drummond beam M. Springolo Page xiii
14 Figure 3.7 Deskovic beam Figure 3.8 Zhao beam Figure 3.9 Van Erp beam Figure 4.1 Stress relations of a ply under a uniform strain Figure 4.2 Anisotropic state of stress Figure 4.3 Strain and stress distributions throughout a beam in bending Figure 4.4 Published momentshear interaction for steel, concrete and composites Figure 4.5 Bearing distribution angle Figure 4.6 Indicative creep modulus versus time (American Society of Civil Engineers 1984, p. 210) Figure 4.7 Indicative creep modulus versus time (Clarke 1996, p. 127) Figure 4.8 Tensile stress rupture of polyester composites (Clarke 1996, p. 128) Figure 4.9 General stress strain relationships of steel and FRP Figure 5.1 Progression of FRP beam designs to alleviate flange buckling Figure 5.2 Placement of core between web laminates Figure 5.3 Rectangular void to reduce stress concentrations under compressive loading Figure 5.4 Exploded view of the beam Figure 5.5 Beam dimensions and designations Figure 5.6 Avery Universal Testing Machine Figure 5.7 Number of unidirectional laminates versus crosssectional area for the FRP beam Figure 5.8 MTS 810 Material Test System Machine Figure 5.9 Nonlinear stress strain behaviour of the PFR in compression Figure 5.10 Nonlinear stress strain behaviour of the PFR in tension Figure 5.11 Form and pour beam production Figure 6.1 FRP beam: load deformation behaviour Figure 6.2 Transformed section of the uncracked FRP beam M. Springolo Page xiv
15 Figure 6.3 Comparison between the use of a constant and variable stiffness of the uncracked FRP beam Figure 6.4 Closeup of cracking with associated debonding Figure 6.5 Transformed section of cracked FRP beam Figure 6.6 Momentcurvature of the FRP beam Figure 6.7 Momentcurvature of the FRP beam, and the Branson model Figure 6.8 Momentcurvature of the FRP beam and the bilinear model Figure 6.9 Some secondary failure modes in bearing Figure 6.10 Stresses upon the web Figure 6.11 Moment buckling of web specimen Figure 6.12 Stresses upon the flange Figure 6.13 Compression buckling of the flange Figure 6.14 Top flange of curved beam: vertical force component Figure 6.15 Secondary forces in flanges and webs Figure 6.16 Standard determination of web dimensions for bearing capacity prediction Figure 6.17 Deformed shape of beam due to the vertical force F w Figure 6.18 Moment diagrams throughout beam section; due to beam curvature (a) and bearing load (b) Figure 6.19 Bearing plate loading Figure 6.20 FEA model crosssection of the FRP beam under bearing load Figure 6.21 FRP beam; shear load deformation behaviour Figure 6.22 Shear stresses throughout the beam crosssection Figure 6.23 Shear correction values throughout the beam Figure 6.24 Exaggerated localised shear dislocation caused by cracking of the PFR Figure 6.25 Principal stresses on the webs Figure 6.26 Shear buckling of web specimen Figure 6.27 Beam in 4point bending Figure 6.28 Principal strains of the transformed FRP beam M. Springolo Page xv
16 Figure 6.29 Momentshear interaction diagrams Figure 6.30 Torsional rotation of the beam Figure 6.31 Lateral buckling behaviour of the FRP beam Figure 6.32 Deflections of a beam undergoing lateral torsional buckling Figure 6.33 Comparison of methods to determine the critical buckling moment of the FRP beam Figure 6.34 Comparison of FEA and analytical solution of the inplane stresses at centre depth of a beam subject to 3point bending Figure 6.35 Stress factor ( D ) as a function of beam depth for an orthotropic beam β Figure 6.36 Effect on capacity by varying top flange core thickness Figure 6.37 Effect on capacity by varying bottom flange core thickness Figure 6.38 Effect on shear and moment capacities by varying web thickness Figure 7.1 B6 strain gauge locations Figure 7.2 Momentstrain relationship of beam B Figure 7.3 Beam geometries Figure 7.4 Loading arrangement of beams Figure 7.5 Loading plates for beam tests Figure 7.6 Typical momentstrain relationship of the test beams Figure 7.7 Momentcurvature relationship of the test beams Figure 7.8 Momentstrain relationship of beam series B Figure 7.9 Momentstrain relationship of beam series B Figure 7.10 Momentstrain relationship of beam series B Figure 7.11 Momentstrain relationship of beam series B Figure 7.12 Momentstrain relationship of beam series B Figure 7.13 Extra reinforcement on web specimen Figure 7.14 Web specimen testing Figure 7.15 Testing web buckling specimen M. Springolo Page xvi
17 Figure 7.16 Failure of web Figure 7.17 Buckling loads of web test strips Figure 7.18 Comparison of beam crushing capacity and analytical solution Figure 7.19 Momentshear testing setup Figure 7.20 Strain gauge rosette arrangement Figure 7.21 Shear loading versus shear strain (normalised based upon maximum values from each series) Figure 7.22 Normalized shear loading versus deflection Figure 7.23 Section geometry of web shear specimens Figure 7.24 Web specimen failure Figure 7.25 Shear stressstrain behaviour of web specimens (inclusive of core) Figure 7.26 Failure of webs in shear and ISO prediction Figure 7.27 Free body diagrams of the initial and final fibre orientation at a crack in the core Figure 7.28 Failure of webs in shear and analytical prediction Figure 7.29 Comparison of ultimate shear capacities and predictions Figure 7.30 Extra reinforcement on web specimen Figure 7.31 Shear buckling of test specimen Figure 7.32 Load versus deformation of shear buckling specimen Figure 7.33 Total deformations of beams Figure 7.34 Moment versus shear Figure 7.35 Torsion testing arrangement Figure 7.36 Beam undergoing torsion testing Figure 7.37 Torsion versus rotation angle Figure 7.38 Test setup for lateral torsional buckling Figure 7.39 Cantilever beam, lateral torsional buckling Figure 7.40 zaxis rotation of cantilever beam Figure 7.41 Failure loads for beams versus model predictions M. Springolo Page xvii
18 Figure 7.42 Failure load and bearing distance of fullysupported series Figure 7.43 Test regime for longterm loading of the beams Figure 7.44 Beams undergoing sustained loading Figure 7.45 Time versus deflection for the three beams tested Figure 7.46 Time versus factor of initial deflection Figure 7.47 Compression flange core thickness versus failure load Figure 7.48 Tension flange core thickness versus failure load Figure 7.49 Web core thickness versus failure load Figure 8.1 Use of thick shell elements results in inaccurate models due to overlapping materials Figure 8.2 Model with orthotropic bricks for flange laminates Figure 8.3 Finite element model of the core with brick elements removed to simulate cracking of a beam in bending Figure 8.4 Comparison of Strand7, analytical solution, and experimental results Figure 8.5 Flow chart of Python script Figure 8.6 FE model versus analytical and experimental results Figure 8.7 FE model versus analytical and experimental results for changing flange core thickness Figure 8.8 Moment buckling of the web specimen Figure 8.9 Modified beam to force punching shear dominant Figure 8.10 Uniformly distributed load on symmetric beam Figure 8.11 FEA results, longitudinal cracking of the core material Figure 8.12 Shear buckling of web specimen Figure 8.13 FEA results, shear stress throughout beam Figure 8.14 Comparison of FE model deflections of the beam under shear loads Figure 8.15 Models of 4point bending Figure 8.16 Comparison of combined loading models Figure 8.17 Comparison between torsion models showing a linear response M. Springolo Page xviii
19 Figure 8.18 Finite element results for first positive eigenvalue Figure 8.19 Comparison of LTB predictions Figure A.1 Measurement of ply in a laminate. (Swanson 1997) Figure B.1 Unidirectional laminate layup sequence Figure B.2 RHS laminate layup Figure B.3 Mandrels and laminates in mould Figure B.4 Pump operation Figure B.5 Injection moulding Figure B.6 Curing cycle Figure C.1 Curvature of beam undergoing pure moment Figure C.2 Laminate orientation Figure C.3 Curved beam, top flange only Figure C.4 Section of top laminate Figure C.5 Flow chart for predicting pure moment behaviour Figure C.6 Shear deformation of a beam segment Figure C.7 Analytical flow chart for shear behaviour Figure C.8 Analytical flow chart for combined shear and moment behaviour (Mohr s circle) Figure C.9 Deflections of a beam undergoing lateral torsional buckling Figure C.10 Force P transformed into the x and y component forces Figure C.11 Flow chart of torsion numerical analysis Figure C.12 Flow chart of lateral torsional buckling analysis Figure E.1 Experimental shear strains series 1 (Experimental results line up with FE ABAQUS) Figure E.2 Experimental shear strains series Figure E.3 Experimental shear strains series Figure E.4 Experimental shear strains series M. Springolo Page xix
20 Figure E.5 Experimental shear strains series Figure E.6 Experimental shear strains series Figure E.7 ms03b Tables Table 2.1 Typical Properties of Cast Thermosets (at 23 C) compiled from Fibre Composite Design and Development Group 1997; Hull & Clyne Table 2.2 Typical properties of cast thermoplastics at 23 C (t=tensile, y=yield) Table 2.3 Properties of typical fibres (Bishop 1989; Hanson 1987) Table 2.4 The properties of FRP laminates, steel, concrete and timber (E. I. dupont de Nemours. 1980; Fiber Science Division of EDO Corp. 1995; Pagano & Hahn 1997; Swanson 1997; Tsai 1986) Table 2.5 Properties of EGlass / West system epoxy (Fibre Composite Design and Development Group 1997) Table 5.1 Nominal beam dimensions Table 5.2 EGlass mat properties Table 5.3 Laminate properties Table 5.4 The properties of PFR Table 7.1 Beam dimensions Table 7.2 Shear test beam dimensions Table 7.3 Shear testing beam spans Table 8.1 Material properties for failure modelling Table 8.2 Moment buckling predictions Table 8.3 FE model indicates that true boundary condition of web is between simplysupported and fixedends restraints Table 8.4 Predictions of punching capacity in modified beam Table 8.5 Predictions of PFR failure within the flanges M. Springolo Page xx
21 Table 8.6 Comparison between web shear models Table 8.7 Shear buckling predictions Table D.1 Buckling specimens Table E.1 ms03b4 results Table E.2 ms03b5 results Table E.3 ms03b6 results Table E.4 ms03b7 results Table E.5 ms03b8 results Table E.6 ms03b9 results Table E.7 Web buckling results, series Table E.8 Web buckling results, series Table E.9 Beam crushing results Table E.10 ms041 tab results Table E.11 ms042 tab results Table E.12 Web shear testing results taking area as total area of specimen Table E.13 Web shear results taking only laminate area into account Table E.14 Web shear specimens including glass stresses Table E.15 ms04b1 beam results Table E.16 ms04b2 beam results Table E.17 ms04b3 beam results Table E.18 ms04b4 beam results Table E.19 ms04b5 beam results Table E.20 ms04b6 beam results Table E.21 Torsion test results Table E.22 Bearing distribution results Table E.23 ms03b1 results M. Springolo Page xxi
22 Nomenclature a γ γ fi γ i M m S s t ε c ε cb.c ε cb.t ε ci ε fci ε fti ε ij ε mb ε mb.cr ε t ε ti θ x θ y κ ν ν i ν f ν w π σ cb σ f σ fci σ fti σ ij σ m σ mb σ mb.cr σ p σ x τ fi Bearing distribution angle (Radians) Absolute shear strain (Radians) Failure shear strain in the laminate i (Radians) Shear strain in the laminate i (Radians) Deformation due to moment loading. (mm) Moment deflection of the beam (mm) Deformation due to shear loading (mm) Shear deflection of the beam (mm) Total deflection of the beam (mm) Compression strain to outer face of beam (mm/mm) Compressive compression buckling strain (mm/mm) Tensile compressive buckling strain (mm/mm) Average compressive strain in laminate i (mm/mm) Compressive failure strain of laminate i (mm/mm) Tensile failure strain of laminate i (mm/mm) Strain on face i in direction j (mm/mm) Moment buckling strain (mm/mm) Critical moment buckling strain (mm/mm) Tensile strain to outer face of beam (mm/mm) Average tensile strain in laminate i (mm/mm) x direction plate rotation component relative to the middle plane (radians) y direction plate rotation component relative to the middle plane (radians) Curvature of a beam (1/mm) Poisson ratio Poisson ratio of laminate i Poisson ratio of the flange. Poisson ratio of web Pi Compressive stress in outer face of column due to buckling. Failure stress of fibres (MPa) Compressive failure stress of laminate i (MPa) Tensile failure stress of laminate i (Mpa) Stress on face i in direction j (Mpa) Failure stress of matrix (MPa) Moment buckling stress (MPa) Critical stress for moment buckling (MPa) Failure stress of ply (MPa) Normal stress in the x direction (Mpa) Failure shear strain of laminate i M. Springolo Page xxii
23 τ fw τ fxyi τ xy τ xyi φ Shear failure stress of the web (Mpa) Failure shear stress of laminate i. (MPa) Shear stress in the xy plane (Mpa) Shear stress of laminate i (MPa) Angle of torsional rotation (radians) φ f Fibre volume fraction (mm 3 /mm 3 ) Fibre volume fraction for laminate i φ fi φ m Matrix volume fraction (mm 3 /mm 3 ) A Crosssectional area of section (mm 2 ) A i Area of laminate i (mm 2 ) A q Quadratic equation coefficient A s Shear area of beam (mm 2 ) A t Area of transformed section (mm 2 ) B Quadratic equation coefficient C Quadratic equation coefficient c Distance from outer tensile face of beam to neutral axis in x direction (mm) c c Distance from outer tensile face of beam to neutral axis in x direction in cracked section (mm) c f Distance from outer tensile face of flange to neutral axis of flange in z direction (mm) CFRP Carbon fibrereinforced polymer C ta Equation constant for core tensile modulus C tb Linear equation coefficient for core tensile modulus c u Distance from outer tensile face of beam to neutral axis in x direction in uncracked section (mm) c y Distance from outer tensile face of beam to neutral axis in y direction (mm) D Overall depth of beam (mm) d Dt f (mm) d b D2t f (mm) d c Dc. (mm) D y Single term for EI E Tensile modulus (MPa) E cc Compression modulus of core material (MPa) E ci Longitudinal compressive modulus of laminate i. (MPa) E ct Tensile modulus of core material (MPa) E f Modulus of fibres (MPa) E f Young s modulus of the flange (MPa) E m Modulus of matrix (MPa) E p Modulus of ply (MPa) E tci Transverse compressive modulus of the laminate i. (MPa) E ti Longitudinal tensile modulus of laminate i (MPa) E tti Transverse tensile modulus of the laminate i. (MPa) E w Young s modulus of Web F Longitudinal force in flange (N) M. Springolo Page xxiii
24 FE FEA F i FRP F w F wc F wc G GFRP Finite Element Finite Element Analysis Longitudinal force in laminate i. (N) FibreReinforced Polymer Transverse compressive force in web (N) Compressive crushing capacity in webs (N) Transverse compressive capacity of web (N) Shear modulus (MPa) Glass fibrereinforced polymer G i Shear modulus of laminate i (MPa) I Second moment of area about x axis (mm 4 ) I c Second moment of area about x axis in cracked section (mm 4 ) I f Second moment of area of flange about the z axis I u Second moment of area about x axis in uncracked section (mm 4 ) I w Second moment of area of web about the z axis I warp Warping constant of the beam I y Second moment of area about y axis (mm 4 ) J Torsion Constant k Timoshenko shear adjustment factor k 1 Compression buckling factor k 2 Plate buckling factor k 3 Shear correction factor L Span of beam specimen (mm) L ef Effective buckling length (mm) L i Laminate i. M Bending Moment (N.mm) M f Bending Moment at failure (N.mm) n i Number of plies in laminate i. P Buckling load (N) P cr Critical buckling load (N) R Radius of curvature (mm) RC Reinforced Concrete RHS Rectangular Hollow Section S Ratio of fibres within a laminate aligned in the direction of force applied t f Overall thickness of flange. (mm) t i Thickness of laminate i. (mm) t pi Thickness of ply in laminate i (mm) t ti Transformed thickness or laminate i for yaxis properties. t w Overall width of web (mm) u xaxis displacement of a plate (mm) v yaxis displacement of a plate (mm) V* Shear force on beam (N) W Overall width of beam (mm) w zaxis displacement of a plate (mm) M. Springolo Page xxiv
25 wc Wc y (mm) w i Width of laminate i. (mm) w ti Transformed width for laminate i for xaxis properties. Z Section modulus (mm 3 ) Degrees Celsius ( C) µm Micrometer GPa Giga Pascals kg Kilograms mm Millimetres MPa Mega Pascals N Newtons Pa Pascals Units Specimen designation The testing specimens used for this study were designated as follows: AAXX AX X Manufacturer Testing Series Specimen type Specimen Number ge = Gary Ellis mh = Mathew Humphreys ms = Mario Springolo 01 = Materials 02 = Delamination 03 = Bending 04 = Shear 05 = Torsion 06 = Lateral torsional buckling 07 = Bearing 08 = Interlaminar / core shear 09 = Combined bending and shear 10 = Web buckling See individual chapters for designations e.g. b1, b2 et cetera 1, 2, 3 et cetera M. Springolo Page xxv
SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationPOSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS
POSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS  Technical Paper  Tidarut JIRAWATTANASOMKUL *1, Dawei ZHANG *2 and Tamon UEDA *3 ABSTRACT The objective of this study is to propose a new
More informationName :. Roll No. :... Invigilator s Signature :.. CS/B.TECH (CENEW)/SEM3/CE301/ SOLID MECHANICS
Name :. Roll No. :..... Invigilator s Signature :.. 2011 SOLID MECHANICS Time Allotted : 3 Hours Full Marks : 70 The figures in the margin indicate full marks. Candidates are required to give their answers
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationSTRESS ANALYSIS OF BONDED JOINTS IN PULTRUDED GRP COMPONENTS
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF BONDED JOINTS IN PULTRUDED GRP COMPONENTS S.W. Boyd*, J. M. DulieuBarton*, O. T. Thomsen**, A.Gherardi* [J.M. DulieuBarton]: janice@soton.ac.uk
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMINE ROOF SUPPORT DESIGN AND ANALYSIS. Document no : Revision no : 1.0
MINE ROOF SUPPORT DESIGN AND ANALYSIS Document no : 1806269723 Revision no : 1.0 DOCUMENT TITLE : MINE ROOF SUPPORT DESIGN AND ANALYSIS DOCUMENT NUMBER : 1806269723 ISSUE : Issue 1.0 DATE : 7 October
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDesign of Beams (Unit  8)
Design of Beams (Unit  8) Contents Introduction Beam types Lateral stability of beams Factors affecting lateral stability Behaviour of simple and built  up beams in bending (Without vertical stiffeners)
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationStructural behaviour of GFRP beams subjected to concentrated loads: experimental tests, numerical modeling and analytical study
Structural behaviour of GFRP beams subjected to concentrated loads: experimental tests, numerical modeling and analytical study Lourenço Almeida Fernandes, IST/DE Civil Abstract: GFRP composites have shown
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More informationSHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXIBLE FIBER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS
SHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXILE FIER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS Hu Shaoqing Supervisor: Susumu KONO ** MEE8165 ASTRACT FRP with low Young
More informationTheory at a Glance (for IES, GATE, PSU)
1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force
More informationENG2000 Chapter 7 Beams. ENG2000: R.I. Hornsey Beam: 1
ENG2000 Chapter 7 Beams ENG2000: R.I. Hornsey Beam: 1 Overview In this chapter, we consider the stresses and moments present in loaded beams shear stress and bending moment diagrams We will also look at
More informationA fatigue design methodology for GRP composites in offshore underwater applications
A fatigue design methodology for GRP composites in offshore underwater applications Dr P. A. FRIEZE P A F A Consulting Engineers Limited, Hampton, Middx, UK INTRODUCTION Norsk Hydro Troll C field  floating
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationLecture03 Design of Reinforced Concrete Members for Flexure and Axial Loads
Lecture03 Design of Reinforced Concrete Members for Flexure and Axial Loads By: Prof. Dr. Qaisar Ali Civil Engineering Department UET Peshawar drqaisarali@uetpeshawar.edu.pk www.drqaisarali.com Prof.
More informationDownloaded from Downloaded from / 1
PURWANCHAL UNIVERSITY III SEMESTER FINAL EXAMINATION2002 LEVEL : B. E. (Civil) SUBJECT: BEG256CI, Strength of Material Full Marks: 80 TIME: 03:00 hrs Pass marks: 32 Candidates are required to give their
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationChapter. Materials. 1.1 Notations Used in This Chapter
Chapter 1 Materials 1.1 Notations Used in This Chapter A Area of concrete crosssection C s Constant depending on the type of curing C t Creep coefficient (C t = ε sp /ε i ) C u Ultimate creep coefficient
More informationLecture04 Design of RC Members for Shear and Torsion
Lecture04 Design of RC Members for Shear and Torsion By: Prof. Dr. Qaisar Ali Civil Engineering Department UET Peshawar drqaisarali@uetpeshawar.edu.pk www.drqaisarali.com 1 Topics Addressed Design of
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationGB/T / ISO 5271:1993
Translated English of Chinese Standard: GB/T1040.12006 www.chinesestandard.net Sales@ChineseStandard.net GB NATIONAL STANDARD OF THE PEOPLE S REPUBLIC OF CHINA ICS 83.080.01 G 31 GB/T 1040.12006 / ISO
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationSRI CHANDRASEKHARENDRA SARASWATHI VISWA MAHAVIDHYALAYA
SRI CHANDRASEKHARENDRA SARASWATHI VISWA MAHAVIDHYALAYA (Declared as Deemedtobe University under Section 3 of the UGC Act, 1956, Vide notification No.F.9.9/92U3 dated 26 th May 1993 of the Govt. of
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationRoadway Grade = m, amsl HWM = Roadway grade dictates elevation of superstructure and not minimum free board requirement.
Example on Design of Slab Bridge Design Data and Specifications Chapter 5 SUPERSTRUCTURES Superstructure consists of 10m slab, 36m box girder and 10m Tgirder all simply supported. Only the design of Slab
More informationBenchmarking study of steelcomposite structures in CAE crash applications. Master s thesis in Applied Mechanics MADELEINE ANDERSSON EMMA LARSSON
Benchmarking study of steelcomposite structures in CAE crash applications Master s thesis in Applied Mechanics MADELEINE ANDERSSON EMMA LARSSON Department of Applied Mechanics CHALMERS UNIVERSITY OF TECHNOLOGY
More informationFinal Analysis Report MIE 313 Design of Mechanical Components
Final Analysis Report MIE 313 Design of Mechanical Components Juliana Amado Charlene Nestor Peter Walsh Table of Contents Abstract:...iii Introduction:... 4 Procedure:... 5 Results:... 6 Reliability:...
More informationAssessment Methods of Mechanical Properties of Composite Materials
Mechanics and Mechanical Engineering Vol. 21, No. 4 (2017) 1005 1018 c Lodz University of Technology Assessment Methods of Mechanical Properties of Composite Materials Monika Kamocka Radoslaw J. Mania
More informationTABLE OF CONTENTS SECTION TITLE PAGE 2 PRINCIPLES OF SEISMIC ISOLATION OF BRIDGES 3
TABLE OF CONTENTS SECTION TITLE PAGE 1 INTRODUCTION 1 2 PRINCIPLES OF SEISMIC ISOLATION OF BRIDGES 3 3 ANALYSIS METHODS OF SEISMICALLY ISOLATED BRIDGES 5 3.1 Introduction 5 3.2 Loadings for the Analysis
More informationMECHANICS OF SOLIDS. (For B.E. Mechanical Engineering Students) As per New Revised Syllabus of APJ Abdul Kalam Technological University
MECHANICS OF SOLIDS (For B.E. Mechanical Engineering Students) As per New Revised Syllabus of APJ Abdul Kalam Technological University Dr. S.Ramachandran, M.E., Ph.D., Mr. V.J. George, M.E., Mr. S. Kumaran,
More informationCHAPTER 6: ULTIMATE LIMIT STATE
CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.
More informationEngineering Science OUTCOME 1  TUTORIAL 4 COLUMNS
Unit 2: Unit code: QCF Level: Credit value: 15 Engineering Science L/601/10 OUTCOME 1  TUTORIAL COLUMNS 1. Be able to determine the behavioural characteristics of elements of static engineering systems
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationTemperature Effects on a Fibre Reinforced Polymer Material
University of Southern Queensland Faculty of Engineering and Surveying Temperature Effects on a Fibre Reinforced Polymer Material A dissertation submitted by Samuel David William Zerbst in fulfilment of
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab
Fatigue Resistance of Angle Shape Shear Connector used in SteelConcrete Composite Slab A dissertation submitted to the Graduate School of Engineering of Nagoya University in partial fulfillment of the
More informationButje Alfonsius Louk Fanggi
AXIAL COMPRESSIVE BEHAVIOR OF FRPCONCRETESTEEL DOUBLESKIN TUBULAR COLUMNS Butje Alfonsius Louk Fanggi BEng and MEng (Structural Engineering) Thesis submitted to The University of Adelaide School of
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationDynamic and buckling analysis of FRP portal frames using a lockingfree finite element
Fourth International Conference on FRP Composites in Civil Engineering (CICE8) 2224July 8, Zurich, Switzerland Dynamic and buckling analysis of FRP portal frames using a lockingfree finite element F.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationCHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS
CHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS S. YanesArmas, J. De Castro and T. Keller Composite Construction Laboratory (CCLab), Ecole Polytechique Fédérale
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More informationN o n l i n e a r M u l t i  S c a l e M o d e l i n g o f A e r o s p a c e C o m p o s i t e s M a t e r i a l s & S t r u c t u r e s
N o n l i n e a r M u l t i  S c a l e M o d e l i n g o f A e r o s p a c e C o m p o s i t e s M a t e r i a l s & S t r u c t u r e s R o g e r A. A s s a k e r C E O, e  X s t r e a m e n g i n e
More informationFOLDING OF WOVEN COMPOSITE STRUCTURES
FOLDING OF WOVEN COMPOSITE STRUCTURES J.C.H. Yee and S. Pellegrino 1 Department of Engineering, University of Cambridge Trumpington Street, Cambridge CB2 1PZ, UK ABSTRACT This paper investigates oneply
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationCHARACTERISATION OF FIBRE GLASS PANELS FOR NAVAL USE
ICEM1212th International Conference on Experimental Mechanics 29 August  2 September, 2004 Politecnico di Bari, Italy CHARACTERISATION OF FIBRE GLASS PANELS FOR NAVAL USE D. Lombardo a, G. Marannano
More informationCIVIL DEPARTMENT MECHANICS OF STRUCTURES ASSIGNMENT NO 1. Brach: CE YEAR:
MECHANICS OF STRUCTURES ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes XX and YY of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationCHAPTER 3 EXPERIMENTAL STUDY
Experimental Study 42 CHAPTER 3 EXPERIMENTAL STUDY 3.1. INTRODUCTION The experimental study that has been carried out in this thesis has two main objectives: 1. Characterise the concrete behaviour in mode
More informationDelhi Noida Bhopal Hyderabad Jaipur Lucknow Indore Pune Bhubaneswar Kolkata Patna Web: Ph:
Serial : IG1_CE_G_Concrete Structures_100818 Delhi Noida Bhopal Hyderabad Jaipur Lucknow Indore Pune Bhubaneswar Kolkata Patna Web: Email: info@madeeasy.in Ph: 011451461 CLASS TEST 01819 CIVIL ENGINEERING
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
The 3 rd International Conerence on DIAGNOSIS AND PREDICTION IN MECHANICAL ENGINEERING SYSTEMS DIPRE 12 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More information